LMucko/crystallography-open-database huggingface dataset:
An X-ray Rietveld study of piemontite on the join Ca2Al3Si3O12(OH) - Ca2Mn3+3Si3O12(OH) formed by hydrothermal synthesis Sample: q = 1.0, p = 1.00, Synthesis at P=200 MPa, T=500 C
Nagashima, M.; Akasaka, M.; American Mineralogist 89 (2004) 1119–1129; doi:

data_9003499
_publ_section_title
;
 An X-ray Rietveld study of piemontite on the join
 Ca2Al3Si3O12(OH) - Ca2Mn3+3Si3O12(OH) formed by hydrothermal synthesis
 Sample: q = 1.0, p = 1.00, Synthesis at P=200 MPa, T=500 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1119
_journal_page_last               1129
_journal_volume                  89
_journal_year                    2004
_chemical_formula_sum            'Al2 Ca2 H Mn O13 Si3'
_chemical_name_mineral           Piemontite
_space_group_IT_number           11
_symmetry_space_group_name_Hall  '-P 2yb'
_symmetry_space_group_name_H-M   'P 1 21/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 115.519
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   8.8531
_cell_length_b                   5.6741
_cell_length_c                   10.1613
_cell_volume                     460.639
_database_code_amcsd             0003589
_diffrn_ambient_pressure         2e+05
_diffrn_ambient_temperature      773.15
_exptl_crystal_density_diffrn    3.477
_cod_original_formula_sum        'Ca2 (Al2 Mn) Si3 O13 H'
_cod_database_code               9003499
An X-ray Rietveld study of piemontite on the join Ca2Al3Si3O12(OH) - Ca2Mn3+3Si3O12(OH) formed by hydrothermal synthesis Sample: q = 1.0, p = 1.00, Synthesis at P=350 MPa, T=500 C
Nagashima, M.; Akasaka, M.; American Mineralogist 89 (2004) 1119–1129; doi:

data_9003500
_publ_section_title
;
 An X-ray Rietveld study of piemontite on the join
 Ca2Al3Si3O12(OH) - Ca2Mn3+3Si3O12(OH) formed by hydrothermal synthesis
 Sample: q = 1.0, p = 1.00, Synthesis at P=350 MPa, T=500 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1119
_journal_page_last               1129
_journal_volume                  89
_journal_year                    2004
_chemical_formula_sum            'Al2 Ca2 H Mn O13 Si3'
_chemical_name_mineral           Piemontite
_space_group_IT_number           11
_symmetry_space_group_name_Hall  '-P 2yb'
_symmetry_space_group_name_H-M   'P 1 21/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 115.499
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   8.8490
_cell_length_b                   5.6670
_cell_length_c                   10.153
_cell_volume                     459.551
_database_code_amcsd             0003590
_diffrn_ambient_pressure         3.5e+05
_diffrn_ambient_temperature      773.15
_exptl_crystal_density_diffrn    3.486
_cod_original_formula_sum        'Ca2 Al2 Mn Si3 O13 H'
_cod_database_code               9003500
An X-ray Rietveld study of piemontite on the join Ca2Al3Si3O12(OH) - Ca2Mn3+3Si3O12(OH) formed by hydrothermal synthesis Sample: q = 1.1, p = 1.04, Synthesis at P=200 MPa, T=500 C
Nagashima, M.; Akasaka, M.; American Mineralogist 89 (2004) 1119–1129; doi:

data_9003501
_publ_section_title
;
 An X-ray Rietveld study of piemontite on the join
 Ca2Al3Si3O12(OH) - Ca2Mn3+3Si3O12(OH) formed by hydrothermal synthesis
 Sample: q = 1.1, p = 1.04, Synthesis at P=200 MPa, T=500 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1119
_journal_page_last               1129
_journal_volume                  89
_journal_year                    2004
_chemical_formula_sum            'Al1.96 Ca2 H Mn1.04 O13 Si3'
_chemical_name_mineral           Piemontite
_space_group_IT_number           11
_symmetry_space_group_name_Hall  '-P 2yb'
_symmetry_space_group_name_H-M   'P 1 21/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 115.503
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   8.8596
_cell_length_b                   5.6834
_cell_length_c                   10.1679
_cell_volume                     462.095
_database_code_amcsd             0003591
_diffrn_ambient_pressure         2e+05
_diffrn_ambient_temperature      773.15
_exptl_crystal_density_diffrn    3.474
_cod_original_formula_sum        'Ca2 (Al1.96 Mn1.04) Si3 O13 H'
_cod_database_code               9003501
An X-ray Rietveld study of piemontite on the join Ca2Al3Si3O12(OH) - Ca2Mn3+3Si3O12(OH) formed by hydrothermal synthesis Sample: q = 1.1, p = 1.03, Synthesis at P=350 MPa, T=500 C
Nagashima, M.; Akasaka, M.; American Mineralogist 89 (2004) 1119–1129; doi:

data_9003502
_publ_section_title
;
 An X-ray Rietveld study of piemontite on the join
 Ca2Al3Si3O12(OH) - Ca2Mn3+3Si3O12(OH) formed by hydrothermal synthesis
 Sample: q = 1.1, p = 1.03, Synthesis at P=350 MPa, T=500 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1119
_journal_page_last               1129
_journal_volume                  89
_journal_year                    2004
_chemical_formula_sum            'Al1.97 Ca2 H Mn1.03 O13 Si3'
_chemical_name_mineral           Piemontite
_space_group_IT_number           11
_symmetry_space_group_name_Hall  '-P 2yb'
_symmetry_space_group_name_H-M   'P 1 21/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 115.511
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   8.860
_cell_length_b                   5.6818
_cell_length_c                   10.167
_cell_volume                     461.914
_database_code_amcsd             0003592
_diffrn_ambient_pressure         3.5e+05
_diffrn_ambient_temperature      773.15
_exptl_crystal_density_diffrn    3.474
_cod_original_formula_sum        'Ca2 (Al1.97 Mn1.03) Si3 O13 H'
_cod_database_code               9003502
An X-ray Rietveld study of piemontite on the join Ca2Al3Si3O12(OH) - Ca2Mn3+3Si3O12(OH) formed by hydrothermal synthesis Sample: q = 1.5, p = 1.26, Synthesis at P=200 MPa, T=500 C
Nagashima, M.; Akasaka, M.; American Mineralogist 89 (2004) 1119–1129; doi:

data_9003503
_publ_section_title
;
 An X-ray Rietveld study of piemontite on the join
 Ca2Al3Si3O12(OH) - Ca2Mn3+3Si3O12(OH) formed by hydrothermal synthesis
 Sample: q = 1.5, p = 1.26, Synthesis at P=200 MPa, T=500 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1119
_journal_page_last               1129
_journal_volume                  89
_journal_year                    2004
_chemical_formula_sum            'Al1.74 Ca2 H Mn1.26 O13 Si3'
_chemical_name_mineral           Piemontite
_space_group_IT_number           11
_symmetry_space_group_name_Hall  '-P 2yb'
_symmetry_space_group_name_H-M   'P 1 21/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 115.540
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   8.8589
_cell_length_b                   5.7017
_cell_length_c                   10.1802
_cell_volume                     463.964
_database_code_amcsd             0003593
_diffrn_ambient_pressure         2e+05
_diffrn_ambient_temperature      773.15
_exptl_crystal_density_diffrn    3.504
_cod_original_formula_sum        'Ca2 (Al1.74 Mn1.26) Si3 O13 H'
_cod_database_code               9003503
An X-ray Rietveld study of piemontite on the join Ca2Al3Si3O12(OH) - Ca2Mn3+3Si3O12(OH) formed by hydrothermal synthesis Sample: q = 1.5, p = 1.25, Synthesis at P=350 MPa, T=500 C
Nagashima, M.; Akasaka, M.; American Mineralogist 89 (2004) 1119–1129; doi:

data_9003504
_publ_section_title
;
 An X-ray Rietveld study of piemontite on the join
 Ca2Al3Si3O12(OH) - Ca2Mn3+3Si3O12(OH) formed by hydrothermal synthesis
 Sample: q = 1.5, p = 1.25, Synthesis at P=350 MPa, T=500 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1119
_journal_page_last               1129
_journal_volume                  89
_journal_year                    2004
_chemical_formula_sum            'Al1.74 Ca2 H Mn1.26 O13 Si3'
_chemical_name_mineral           Piemontite
_space_group_IT_number           11
_symmetry_space_group_name_Hall  '-P 2yb'
_symmetry_space_group_name_H-M   'P 1 21/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 115.525
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   8.8625
_cell_length_b                   5.7006
_cell_length_c                   10.1822
_cell_volume                     464.212
_database_code_amcsd             0003594
_diffrn_ambient_pressure         3.5e+05
_diffrn_ambient_temperature      773.15
_exptl_crystal_density_diffrn    3.503
_cod_original_formula_sum        'Ca2 (Al1.74 Mn1.26) Si3 O13 H'
_cod_database_code               9003504
An X-ray Rietveld study of piemontite on the join Ca2Al3Si3O12(OH) - Ca2Mn3+3Si3O12(OH) formed by hydrothermal synthesis Sample: q = 1.75, p = 1.26, Synthesis at P=200 MPa, T=500 C
Nagashima, M.; Akasaka, M.; American Mineralogist 89 (2004) 1119–1129; doi:

data_9003505
_publ_section_title
;
 An X-ray Rietveld study of piemontite on the join
 Ca2Al3Si3O12(OH) - Ca2Mn3+3Si3O12(OH) formed by hydrothermal synthesis
 Sample: q = 1.75, p = 1.26, Synthesis at P=200 MPa, T=500 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1119
_journal_page_last               1129
_journal_volume                  89
_journal_year                    2004
_chemical_formula_sum            'Al1.75 Ca2 H Mn1.25 O13 Si3'
_chemical_name_mineral           Piemontite
_space_group_IT_number           11
_symmetry_space_group_name_Hall  '-P 2yb'
_symmetry_space_group_name_H-M   'P 1 21/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 115.548
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   8.8591
_cell_length_b                   5.7039
_cell_length_c                   10.1827
_cell_volume                     464.236
_database_code_amcsd             0003595
_diffrn_ambient_pressure         2e+05
_diffrn_ambient_temperature      773.15
_exptl_crystal_density_diffrn    3.500
_cod_original_formula_sum        'Ca2 (Al1.75 Mn1.25) Si3 O13 H'
_cod_database_code               9003505
An X-ray Rietveld study of piemontite on the join Ca2Al3Si3O12(OH) - Ca2Mn3+3Si3O12(OH) formed by hydrothermal synthesis Sample: q = 1.75, p = 1.25, Synthesis at P=350 MPa, T=500 C
Nagashima, M.; Akasaka, M.; American Mineralogist 89 (2004) 1119–1129; doi:

data_9003506
_publ_section_title
;
 An X-ray Rietveld study of piemontite on the join
 Ca2Al3Si3O12(OH) - Ca2Mn3+3Si3O12(OH) formed by hydrothermal synthesis
 Sample: q = 1.75, p = 1.25, Synthesis at P=350 MPa, T=500 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1119
_journal_page_last               1129
_journal_volume                  89
_journal_year                    2004
_chemical_formula_sum            'Al1.75 Ca2 H Mn1.25 O13 Si3'
_chemical_name_mineral           Piemontite
_space_group_IT_number           11
_symmetry_space_group_name_Hall  '-P 2yb'
_symmetry_space_group_name_H-M   'P 1 21/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 115.518
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   8.8581
_cell_length_b                   5.6949
_cell_length_c                   10.1771
_cell_volume                     463.312
_database_code_amcsd             0003596
_diffrn_ambient_pressure         3.5e+05
_diffrn_ambient_temperature      773.15
_exptl_crystal_density_diffrn    3.507
_cod_original_formula_sum        'Ca2 (Al1.75 Mn1.25) Si3 O13 H'
_cod_database_code               9003506
Incorporation of sodium into the chlorite structure: the crystal structure of glagolevite, Na(Mg,Al)6[Si3AlO10](OH,O)8
Krivovichev, S. V.; Armbruster, T.; Organova, N. I.; Burns, P. C.; Seredkin, M. V.; Chukanov, N. V.; American Mineralogist 89 (2004) 1138–1141; doi:

data_9003507
_publ_section_title
;
 Incorporation of sodium into the chlorite structure: the crystal structure
 of glagolevite, Na(Mg,Al)6[Si3AlO10](OH,O)8
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1138
_journal_page_last               1141
_journal_volume                  89
_journal_year                    2004
_chemical_formula_sum            'H2 Mg2 Na0.193 O6 Si1.333'
_chemical_name_mineral           Glagolevite
_space_group_crystal_system      triclinic
_space_group_IT_number           1
_space_group_name_Hall           'C 1'
_space_group_name_H-M_alt        'C 1'
_symmetry_space_group_name_H-M   'C 1'
_cell_angle_alpha                90.00
_cell_angle_beta                 97.08
_cell_angle_gamma                90.00
_cell_length_a                   5.3580
_cell_length_b                   9.2810
_cell_length_c                   14.574
_cell_formula_units_Z            6
_cell_volume                     719.204
_database_code_amcsd             0003597
_exptl_crystal_density_diffrn    2.612
_cod_original_formula_sum        'Mg2 Na.193 Si1.333 O6 H2'
_cod_database_code               9003507
Cation disorder in dolomite, CaMg(CO3)2, and its influence on the aragonite+magnesite - dolomite reaction boundary Sample: P = 3 GPa, T = 296 K
Antao, S. M.; Mulder, W. H.; Hassan, I.; Crichton, W. A.; Parise, J. B.; American Mineralogist 89 (2004) 1142–1147; doi:

data_9003508
_publ_section_title
;
 Cation disorder in dolomite, CaMg(CO3)2, and its influence on the
 aragonite+magnesite - dolomite reaction boundary
 Sample: P = 3 GPa, T = 296 K
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1142
_journal_page_last               1147
_journal_volume                  89
_journal_year                    2004
_chemical_formula_sum            'C2 Ca Mg O6'
_chemical_name_mineral           Dolomite
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.8072
_cell_length_b                   4.8072
_cell_length_c                   16.0048
_cell_formula_units_Z            3
_cell_volume                     320.306
_database_code_amcsd             0003598
_diffrn_ambient_pressure         3e+06
_diffrn_ambient_temperature      296
_exptl_crystal_density_diffrn    2.868
_cod_original_sg_symbol_H-M      'R -3'
_cod_original_formula_sum        'Ca Mg C2 O6'
_cod_database_code               9003508
Cation disorder in dolomite, CaMg(CO3)2, and its influence on the aragonite+magnesite - dolomite reaction boundary Sample: P = 3 GPa, T = 630 K
Antao, S. M.; Mulder, W. H.; Hassan, I.; Crichton, W. A.; Parise, J. B.; American Mineralogist 89 (2004) 1142–1147; doi:

data_9003509
_publ_section_title
;
 Cation disorder in dolomite, CaMg(CO3)2, and its influence on the
 aragonite+magnesite - dolomite reaction boundary
 Sample: P = 3 GPa, T = 630 K
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1142
_journal_page_last               1147
_journal_volume                  89
_journal_year                    2004
_chemical_formula_sum            'C Ca0.5 Mg0.5 O3'
_chemical_name_mineral           Dolomite
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            6
_cell_length_a                   4.7924
_cell_length_b                   4.7924
_cell_length_c                   15.8119
_cell_volume                     314.500
_database_code_amcsd             0003599
_diffrn_ambient_pressure         3e+06
_diffrn_ambient_temperature      630
_exptl_crystal_density_diffrn    2.921
_cod_original_sg_symbol_H-M      'R -3'
_cod_original_formula_sum        '(Ca.5 Mg.5) C O3'
_cod_database_code               9003509
Cation disorder in dolomite, CaMg(CO3)2, and its influence on the aragonite+magnesite - dolomite reaction boundary Sample: P = 3 GPa, T = 675 K
Antao, S. M.; Mulder, W. H.; Hassan, I.; Crichton, W. A.; Parise, J. B.; American Mineralogist 89 (2004) 1142–1147; doi:

data_9003510
_publ_section_title
;
 Cation disorder in dolomite, CaMg(CO3)2, and its influence on the
 aragonite+magnesite - dolomite reaction boundary
 Sample: P = 3 GPa, T = 675 K
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1142
_journal_page_last               1147
_journal_volume                  89
_journal_year                    2004
_chemical_formula_sum            'C Ca0.5 Mg0.5 O3'
_chemical_name_mineral           Dolomite
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            6
_cell_length_a                   4.7918
_cell_length_b                   4.7918
_cell_length_c                   15.8283
_cell_volume                     314.747
_database_code_amcsd             0003600
_diffrn_ambient_pressure         3e+06
_diffrn_ambient_temperature      675
_exptl_crystal_density_diffrn    2.919
_cod_original_sg_symbol_H-M      'R -3'
_cod_original_formula_sum        '(Ca.5 Mg.5) C O3'
_cod_database_code               9003510
Cation disorder in dolomite, CaMg(CO3)2, and its influence on the aragonite+magnesite - dolomite reaction boundary Sample: P = 3 GPa, T = 809 K
Antao, S. M.; Mulder, W. H.; Hassan, I.; Crichton, W. A.; Parise, J. B.; American Mineralogist 89 (2004) 1142–1147; doi:

data_9003511
_publ_section_title
;
 Cation disorder in dolomite, CaMg(CO3)2, and its influence on the
 aragonite+magnesite - dolomite reaction boundary
 Sample: P = 3 GPa, T = 809 K
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1142
_journal_page_last               1147
_journal_volume                  89
_journal_year                    2004
_chemical_formula_sum            'C Ca0.5 Mg0.5 O3'
_chemical_name_mineral           Dolomite
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            6
_cell_length_a                   4.7917
_cell_length_b                   4.7917
_cell_length_c                   15.8816
_cell_volume                     315.794
_database_code_amcsd             0003601
_diffrn_ambient_pressure         3e+06
_diffrn_ambient_temperature      809
_exptl_crystal_density_diffrn    2.909
_cod_original_sg_symbol_H-M      'R -3'
_cod_original_formula_sum        '(Ca.5 Mg.5) C O3'
_cod_database_code               9003511
Cation disorder in dolomite, CaMg(CO3)2, and its influence on the aragonite+magnesite - dolomite reaction boundary Sample: P = 3 GPa, T = 925 K
Antao, S. M.; Mulder, W. H.; Hassan, I.; Crichton, W. A.; Parise, J. B.; American Mineralogist 89 (2004) 1142–1147; doi:

data_9003512
_publ_section_title
;
 Cation disorder in dolomite, CaMg(CO3)2, and its influence on the
 aragonite+magnesite - dolomite reaction boundary
 Sample: P = 3 GPa, T = 925 K
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1142
_journal_page_last               1147
_journal_volume                  89
_journal_year                    2004
_chemical_formula_sum            'C Ca0.5 Mg0.5 O3'
_chemical_name_mineral           Dolomite
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            6
_cell_length_a                   4.7925
_cell_length_b                   4.7925
_cell_length_c                   15.9312
_cell_volume                     316.886
_database_code_amcsd             0003602
_diffrn_ambient_pressure         3e+06
_diffrn_ambient_temperature      925
_exptl_crystal_density_diffrn    2.899
_cod_original_sg_symbol_H-M      'R -3'
_cod_original_formula_sum        '(Ca.5 Mg.5) C O3'
_cod_database_code               9003512
Cation disorder in dolomite, CaMg(CO3)2, and its influence on the aragonite+magnesite - dolomite reaction boundary Sample: P = 3 GPa, T = 999 K
Antao, S. M.; Mulder, W. H.; Hassan, I.; Crichton, W. A.; Parise, J. B.; American Mineralogist 89 (2004) 1142–1147; doi:

data_9003513
_publ_section_title
;
 Cation disorder in dolomite, CaMg(CO3)2, and its influence on the
 aragonite+magnesite - dolomite reaction boundary
 Sample: P = 3 GPa, T = 999 K
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1142
_journal_page_last               1147
_journal_volume                  89
_journal_year                    2004
_chemical_formula_sum            'C Ca0.5 Mg0.5 O3'
_chemical_name_mineral           Dolomite
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            6
_cell_length_a                   4.7938
_cell_length_b                   4.7938
_cell_length_c                   15.9652
_cell_volume                     317.735
_database_code_amcsd             0003603
_diffrn_ambient_pressure         3e+06
_diffrn_ambient_temperature      999
_exptl_crystal_density_diffrn    2.891
_cod_original_sg_symbol_H-M      'R -3'
_cod_original_formula_sum        '(Ca.5 Mg.5) C O3'
_cod_database_code               9003513
Cation disorder in dolomite, CaMg(CO3)2, and its influence on the aragonite+magnesite - dolomite reaction boundary Sample: P = 3 GPa, T = 1039 K
Antao, S. M.; Mulder, W. H.; Hassan, I.; Crichton, W. A.; Parise, J. B.; American Mineralogist 89 (2004) 1142–1147; doi:

data_9003514
_publ_section_title
;
 Cation disorder in dolomite, CaMg(CO3)2, and its influence on the
 aragonite+magnesite - dolomite reaction boundary
 Sample: P = 3 GPa, T = 1039 K
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1142
_journal_page_last               1147
_journal_volume                  89
_journal_year                    2004
_chemical_formula_sum            'C Ca0.5 Mg0.5 O3'
_chemical_name_mineral           Dolomite
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            6
_cell_length_a                   4.7941
_cell_length_b                   4.7941
_cell_length_c                   15.9868
_cell_volume                     318.205
_database_code_amcsd             0003604
_diffrn_ambient_pressure         3e+06
_diffrn_ambient_temperature      1039
_exptl_crystal_density_diffrn    2.887
_cod_original_cell_volume        318.204
_cod_original_sg_symbol_H-M      'R -3'
_cod_original_formula_sum        '(Ca.5 Mg.5) C O3'
_cod_database_code               9003514